0

**RESEARCH PAPER **

**Evaluation of the flexural strength and serviceability of geopolymer **

**concrete beams reinforced with Glass-Fibre-Reinforced Polymer (GFRP) **

**bars **

(Title contains 17 words)

Running headline: Evaluation of the flexural strength and serviceability of geopolymer concrete beams reinforced with Glass-Fibre-Reinforced Polymer (GFRP) bars (126 characters)

by

**G.B. Maranan1 _{, A.C. Manalo}1_{, B. Benmokrane}2_{, W. Karunasena}1_{, and P. Mendis}3 **

1_{ Centre of Excellence in Engineered Fibre Composites (CEEFC), }

Faculty of Health, Engineering and Sciences (FoHES), University of Southern Queensland, Toowoomba 4350, Australia

2_{ Department of Civil Engineering, University de Sherbrooke, Sherbrooke, Quebec, }

Canada J1K 2R1

3_{ Department of Infrastructure Engineering, The University of Melbourne, Victoria 3010, }

Australia

Submitted to
**Engineering Structures **

Corresponding Author:

**Allan Manalo **

Senior Lecturer in Civil Engineering (Structural)

Centre of Excellence in Engineered Fibre Composites (CEEFC), Faculty of Health, Engineering and Sciences,

University of Southern Queensland, Toowoomba, Queensland 4350, Australia Tel: +61 7 4631 2547 Fax: +61 7 4631 2110

E-mail: allan.manalo@usq.edu.au

**Manuscript summary: **

Total pages 29 (including 1-page cover) Number of figures 8

1

**Evaluation of the flexural strength and serviceability of geopolymer **

**concrete beams reinforced with Glass-Fibre-Reinforced Polymer (GFRP) **

**bars **

**G.B. Maranan1 _{, A.C. Manalo}1,*_{, B. Benmokrane}2_{, W. Karunasena}1_{, and P. Mendis}3 **

1_{ Centre of Excellence in Engineered Fibre Composites (CEEFC), Faculty of Health, Engineering and Sciences }

(FoHES), University of Southern Queensland, Toowoomba 4350, Australia

2_{ Department of Civil Engineering, University de Sherbrooke, Sherbrooke, Quebec, Canada J1K 2R1 }

3_{ Department of Infrastructure Engineering, The University of Melbourne, Victoria 3010, Australia }

Email: ginghis.maranan@usq.edu.au; allan.manalo@usq.edu.au; bbenmokrane@andrew.sca.usherb.ca;

karu.karunasena@usq.edu.au; pamendis@unimelb.edu.au

**Abstract **

2
**Keywords: ** Geopolymer concrete; glass-fiber-reinforced polymer (GFRP) bars; Flexural
strength; Serviceability; Effective bond; FRP-reinforced concrete.

_________________________ *Corresponding author, tel. +61 7 4631 2547; fax. +61 7 4631 2110 E-mail addresses: allan.manalo@usq.edu.au (A. C. Manalo)

**1. Introduction **

Reinforced concrete (RC) is one of the most commonly used composite materials in the construction of roads, bridges, buildings, and other civil infrastructures. The demand for this material is expected to increase in the future owing to the rise of infrastructure needs in many developing and industrialised countries. In fact, it is estimated that the total global infrastructure demand amounts to USD 4.0 trillion with a gap of at least USD 1.0 trillion per year [1]. Due to the serviceability and economic issues owing to the costly repair and rehabilitation of damaged RC structures caused by the corrosion of the steel bars and the sustainability issue owing to the extremely resource- and energy-intensive process of producing steel and cement materials, however, many engineers and researchers have sought viable alternatives. Among the solutions that are currently being employed are replacing cement-based concrete with geopolymer concrete and replacing steel bars with fibre-reinforced polymer (FRP) bars. Neither, however, can solve the issues altogether.

3 and sustainable construction system. As the demand for the rehabilitation of existing RC structures and the construction of new infrastructure increases, accompanied with the mounting fly-ash production mainly in China, India and Australia [9], there is an urgent need for a thorough investigation of the proposed system so as to increase its uptake in the construction industry.

Generally, the behaviour of concrete beams reinforced with FRP bars (FRP-RC) is different from the traditional RC beams in many ways, mainly because of the differences between the physical and mechanical properties of FRP and steel reinforcements [10]. First, FRP-RC beams exhibit lower serviceability performance owing to the lower modulus of elasticity of FRP bars compared to steel bars [11-13]. Secondly, FRP-RC beams are usually designed as over-reinforced because concrete crushing failure is less brittle and less catastrophic compared to FRP rupture failure owing to the rigid and brittle behaviour of FRP bars. Lastly, since the surface geometries and mechanical features of FRP bars are different from steel bars, they bond differently to concrete than steel bars. Some researchers [14-16] predicted the structural behaviour of the FRP-RC system using the existing equations developed for the conventional RC with some modifications to account for these differences.

4 paste [9]. Even though the strength is different, the load-deflection characteristics, crack patterns, and failure modes of RGC beams are analogous to RC beams [18, 19].

While there are numerous references in the literature about the strength and serviceability performance of FRP-RC and S-RGC beams, few studies have investigated the behaviour of geopolymer concrete beams reinforced with FRP bars, which is the novelty of this research. The direct pullout test conducted by Maranan et al. [20] showed an adequate bond between glass-fibre-reinforced polymer (GFRP) bars and geopolymer concrete resulting from the mechanical interlock and friction force provided by the sand coating on the surface of the GFRP bars indicating their suitability as reinforcement to geopolymer concrete. In this study, the strength and serviceability performance of the geopolymer concrete beams reinforced with GFRP bars were evaluated with a four-point static bending test. The parameters investigated were the nominal bar diameter, the reinforcement ratio, and the anchorage system.

**2. Experimental Program **

**2.1. Materials **

*2.1.1. Geopolymer Concrete *

5 Furthermore, the modulus of rupture test of four geopolymer concrete prisms with a cross-sectional area of 75 mm by 75 mm and a length 250 mm yielded an average value of 3.86 MPa. This value was computed using Equation 7 in Table 8.

*2.1.2. GFRP Bars *

The GFRP bars used in this study were provided by V-ROD® Australia [8] and were manufactured by pultrusion process of E-glass fibres impregnated in modified vinyl ester resin. High modulus (HM) GFRP bars (Grade III, CSA S807-10) of varying nominal diameters were considered in this study (Figure 2): 12.7 mm, 15.9 mm, and 19.0 mm nominal diameter sand-coated GFRP bars with fibre contents in percent by weight of 84.1, 83.9, and 84, respectively [21]. Straight (without anchor head) and headed (with anchor head) GFRP bars were used to investigate the influence of the anchorage system on the flexural behaviour of the specimens. The guaranteed properties of GFRP bars as reported by the manufacturer [21] are given in Table 1. The tensile strength and elastic modulus were calculated using nominal cross-sectional area. For the purpose of comparison, 16.0 mm deformed steel bars were utilised as longitudinal reinforcement in one of the tested beams. Table 2 presents the mechanical properties of the steel bar.

**2.2. Test Specimens **

6
longitudinal tensile reinforcement ratio, and anchorage system. Table 3 summarises the label
and classification of the tested beams. The specimens were designated based on the type and
amount of bottom longitudinal reinforcement. The first two letters indicate the reinforcement
type such as SG for straight GFRP bars (without anchor head), HG for headed GFRP bars (with
anchor head), and DS for deformed steel bars. The abbreviation RGC stands for “reinforced
geopolymer concrete” followed by a numeral that specifies the number of bottom bars. The last
numeral represents the corresponding nominal bar diameter. For example, the specimen
identified as SG-RGC-2-19.0 means that it is a geopolymer concrete beam reinforced with two
19.0 mm diameter straight GFRP bars. In this study, Equations 1 (3) and 2 (4), recommended
by CSA-S806-12 [22] and ACI 440.1R-06 [23] (ACI 318-08 [24]), were used to calculate the
actual reinforcement ratios ρ*f* (ρ*s*) and the balanced reinforcement ratios ρ*fb* (ρ*b*), respectively,
of the geopolymer concrete beams reinforced with GFRP bars (steel bars). Table 8 provides
these equations. The equivalent rectangular stress-block factors, α*1* and β*1*, were calculated
from Equation 5 for CSA code and from Equation 6 for ACI code, both equations can be found
also in Table 8. SG-RGC and HG-RGC beams were designed as over-reinforced (ρ*f */ρ*fb* > 1.0),
while DS-RGC beam was designed as under-reinforced (ρ*s */ρ*b* < 1.0). The ultimate strains were
assumed equivalent to 0.0035 and 0.003, as per CSA and ACI, respectively.

**2.3. Test Setup and Procedure **

7 beams were instrumented with electrical-resistance strain gauges at midspan—bonded to the top surface of the geopolymer concrete and on the top and bottom reinforcement—to measure the longitudinal strains during loading. The strain gauges and sensor were connected to a data-acquisition unit to record their readings continuously.

**3. Test Results and Observations **

This section summarises the experimental results, including the load–deflection relationship, mode of failure, flexural capacity, midspan deflection, strains in the bars and geopolymer concrete, and cracking behaviour of the tested beams.

**3.1. Load–Deflection Relationship **

8 compression zone. The observed nonlinearity was caused by either the extensive cracking at the bottom or the extensive crushing of the geopolymer concrete and not due to yielding of GFRP bars [27, 28]. As the figure shows, the stiffness of the second segment is similar for beams with the same reinforcement ratio. The slope, however, increases as the amount of reinforcement increases. These findings seem to be consistent with the results obtained in FRP-reinforced concrete beams [26, 29, 30]. Afterwards, a sudden load drop occurred, indicating that concrete crushing failure had transpired. Interestingly, the beams did not readily lose their load-carrying capacity after this failure; instead, they continued to sustain additional loads. This behaviour can be attributed to the confinement effect provided by the GFRP stirrups that enhanced the beam ductility and strength. This section represents the third segment of the curve, which has a lower flexural stiffness owing to the initiation of failure in GFRP bars. To avoid any mishaps, the maximum applied load was limited to a magnitude marginally lower than the capacity of the load applicator. Similarly, the behaviour during load removal was recorded to create an unloading curve. This tends to show the elastic characteristic of the beams at higher loads, even after exhibiting nonlinear behaviour or even after the concrete crushing failure. On the other hand, the load–deflection relationship of HG-RGC is comparable to that of SG-RGC with similar amount of reinforcements. Noting that the bars are fully bonded in geopolymer concrete, this result corroborates with the findings of Maranan et al. [31] , which stated that, as the embedment length increases, the bond strength of the straight and headed GFRP bars become analogous to each other.

9 HG-RGC did not exhibit this plastic behaviour. Upon the removal of the applied load, an unyielding curve occurred, but the residual deflection of this beam was much higher than that of SG-RGC and HG-RGC.

**3.2. Mode of Failure **

Table 4 summarises the observed failure modes of the tested beams. As depicted in Figure 6, the over-reinforced SG-RGC and HG-RGC failed in flexure due to geopolymer concrete crushing in the compression zone. The ACI 440.1R-06 and CSA S806-12 codes recommend this mode of failure for any concrete beams reinforced with FRP bars since this type of failure is more gradual, less brittle, and less catastrophic with higher deformability compared to the tensile rupture of FRP bars [32, 33]. On the other hand, Figure 7 shows that the under-reinforced DS-RGC also failed in flexure but steel yielding induced the failure. Since all the tested beams failed according to their intended failure, it can be deduced that the beams were designed satisfactorily.

**3.3. Flexural Capacity **

*3.3.1. Cracking moment *

The loads at which the first crack appeared were recorded during the experiment and were
verified from the load–deflection and moment–strain relationships. Table 4 presents the
experimental cracking moment M*cr-exp* of the tested beams. Nearly similar M*cr-exp* values were
obtained because this parameter mainly depends on the geopolymer concrete tensile strength.
The average M*cr-exp* was 10.9 kN-m that translates to a modulus of rupture f*r* of 3.64 MPa, which
is comparable to the f*r* (3.86 MPa) of the geopolymer concrete prisms.

10
In this study, two benchmarks were employed to determine the bending-moment capacity at
service condition M*s-exp*. The first criterion was based on ISIS-07 [34], which defines the M*s-exp *
as the bending-moment that corresponds to a tensile-strain of 2000 με in the reinforcement.
Using this principle, the M*s-exp *of SG-RGC and HG-RGC were relatively comparable with each
other with an average value of 26.2 kN-m. The M*s-exp *of DS-RGC, however, was 1.85 times
higher than that of SG-RGC and HG-RGC because of the higher elastic modulus of steel bars
compared with GFRP bars. The second criterion was based on Bischoff et al.’s [35]
recommendation wherein the M*s-exp *is approximated as 30% of the beam’s bending-moment
capacity at failure (0.3M*u-exp*). All beams reinforced with GFRP bars, except SG-RGC-2-19.0,
recorded comparable M*s-exp values. Based on this criterion, however, DS-RGC yielded a lower *

*Ms-exp* compared with SG-RGC and HG-RGC due to its lower M*u-exp*.

*3.3.3. At failure *

Table 4 provides the experimental bending-moment capacity M*u-exp* of SG-RGC and HG-RGC
at geopolymer concrete crushing failure and of DS-RGC at steel yielding. The M*u-exp* of
RGC-2-19.0 (91.4 kN-m), RGC-3-15.9 (104.8 kN-m), RGC-4-12.7 (96.1 kN-m),
SG-RGC-5-15.9 (99.3kN-m), and HG-RGC-3-15.9 105.0 kN-m were relatively equivalent to each
other. The slight variation can be attributed to the intrinsic nonhomogeneous and anisotropic
characteristic of the geopolymer concrete. On the other hand, the early yielding of steel bars
prior to geopolymer concrete crushing failure resulted in a lower M*u-exp* for DS-RGC-3-16.0
(85.4kN-m) compared with SG-RGC and HG-RGC having similar ρ*f*, thereby showing the
superiority of the GFRP bars over the steel bars in terms of load-carrying capacity.

*3.3.4. At peak *

All the tested beams continued to carry additional loads after the concrete crushing failure,
yielding another peak named as peak bending-moment capacity M*peak-exp* in this study. The

11
kN-m, and 109.3kN-m, respectively. The initial 25 mm gap between the beam and the load
applicator yielded a relatively lower M*peak-exp* for SG-RGC-3-15.9 compared with the other
beams. The 113.8 kN-m and 118.9 kN-m M*peak-exp* of HG-RGC-3-15.9 and SG-RGC-5-15.9
were slightly higher than that of SG-RGC-3-15.9. Nevertheless, the M*peak-exp* of the former
beams could be much higher than that of the latter beam if the beams were taken to final failure.
On the other hand, the M*peak-exp* achieved by DS-RGC-3-16.0 (74.2 kN-m) was much lower
compared to SG-RGC beams of similar ρ*f*.

**3.4. Midspan Deflection **
*3.4.1. At service load *

Table 5 summarises the immediate midspan deflection at service condition Δ*s-exp* of the tested
beams. The ISIS-07 criterion-based Δ*s-exp* were 8.7 mm, 7.1 mm, and 10.6 mm for
SG-RGC-2-19.0, SG-RGC-3-15.9, and SG-RGC-4-12.7, respectively, while the Δ*s-exp* based from
Bischoff’s recommendation were 8.8 mm, 12.3 mm, and 11.5 mm, respectively. Generally,
comparable results were obtained for each criterion. The Δ*s-exp *(7.3 mm and 8.0 mm based on
ISIS-07 and Bischoff, respectively) of RGC-5-15.9 was generally lower than that of
SG-RGC with lower ρ*f*. HG-RGC-3-15.9, on the other hand, yielded similar Δ*s-exp as SG-RGC with *
comparable *ρf*, 10.0 mm based on ISIS-07 and 11.3 mm based on Bischoff’s criterion. In
general, the Δ*s-exp* from Bischoff’s recommendation were more conservative than that of
ISIS-07 in terms of deflection limits set by ACI 440.1R-06 and CSA S806-12 (L/240 or 10.8 mm).
Thus, the criterion set by Bischoff should be used as the basis for designing GFRP-reinforced
geopolymer concrete beams. The Δ*s-exp* of DS-RGC-3-16.0 was generally higher than that of its
SG-RGC counterparts.

12
The measured Δ*u-exp *of SG-RGC-2-19.0, SG-RGC-3-15.9, and SG-RGC-4-12.7 were 43.4 mm,
52.5 mm, and 53.2 mm, respectively. Except for SG-RGC-2-19.0, the recorded deflections
were almost analogous with each other. SG-RGC-5-15.9 yielded a lower Δ*u-exp *(42.0 mm)
compared with the other beams due to its higher stiffness, owed to its higher amount of
reinforcements. This finding was also observed by Yoo et al. [30]. The Δ*u-exp* of
HG-RGC-3-15.9 (54.1 mm) was nearly comparable to SG-RGC with similar reinforcement ratios. The Δ

*u-exp* (28.4 mm) of the DS-RGC beam is much lower than that of the SG-RGC.

*3.4.3. At the unloading phase *

After removing the applied load, all the beams reinforced with GFRP bars tended to return to
their original position. The residual deflections, Δ*res-exp*, of SG-RGC were comparable to that
of the HG-RGC beam, approximately equivalent to 14 mm. This finding proves the effective
flexural bond of the sand-coated GFRP bars in the geopolymer concrete. Furthermore, it also
shows the inherent elastic behaviour of the SG-RGC, mainly because of the partial
development of the tensile strength of the GFRP bars. The Δ*res-exp * of DS-RGC was
approximately four times higher than that of SG-RGC owing to the inelastic yielding of the
steel bars.

**3.5. Strain Distribution **

13 and nonlinear segments with reduced slope after cracking, and a nonlinear segment after the crushing failure of the geopolymer concrete. The moment–strain curves of the geopolymer concrete in compression zone consisted only of the first two segments since the strain gauges were damaged after the crushing failure. The top GFRP bars, however, continued to provide strain readings. This can be due to the confinement effect provided by the stirrups that protected the bars from buckling and/or kinking.

Table 6 summarises the bar and concrete strains at service condition as defined by Bischoff, at concrete crushing failure, and at peak load. SG-RGC with similar reinforcement ratios yielded nearly comparable strains at different load stages. The tabulated values make it clear, however, that increasing the reinforcement ratio would generally result in lower strains at the bottom GFRP bars. The strain readings at service condition of DS-RGC were generally lower than that of SG-RGC.

**3.6. Cracking Behaviour **

14 the geopolymer concrete. Furthermore, all the beams experienced significant flexural cracking before the inclined cracks joined the flexural cracks, thereby assuring that the beams failed in flexure and not in shear.

15
Comparable crack patterns were observed between SG-RGC and HG-RGC with similar
*ρf*. The figure also demonstrates that the anchor heads have no significant influence on beam
cracking behaviour and that an adequate bond can be secured with sand coating alone.

**4. Discussion **

This section summarises the influence of the nominal bar diameter, reinforcement ratio, and anchorage system on the flexural performance of the geopolymer concrete beams reinforced with GFRP bars. A comparison between the experimental and theoretical results was also presented in this section. The published results on FRP-reinforced concrete beams were compared with the experimental results.

**4.1. Influence of the Nominal Bar Diameter **

This study utilised 12.7 mm, 15.9 mm, and 19.0 mm GFRP bars as longitudinal reinforcement for geopolymer concrete beams. Based on the experimental results, the nominal bar diameter had no significant effect on the flexural strength and serviceability performance of the geopolymer concrete beams reinforced with sand-coated GFRP bars. Generally, SG-RGC-2-19.0, SG-RGC-3-15.9, and SG-RGC-4-12.7 yielded similar flexural strengths, load–deflection characteristics, crack patterns, and deflections. The comparable behaviour of these beams can be expected, since these beams were designed as over-reinforced and consequently, their flexural behaviour would mainly depend on the properties of the geopolymer concrete and not on the diameter of the GFRP bars. Furthermore, noting that all the tested beams were manufactured with a single batch of geopolymer concrete, it can expected that beams with similar reinforcement ratios would yield similar flexural performance.

16
The flexural stiffness of the beams after cracking or the slope of the second segment of their
load-deflection curves increases as the reinforcement ratio increases. Thus, it can be deduced
from the experimental results that the serviceability performance of a GFRP-reinforced
geopolymer concrete beam can be enhanced by increasing the amount of longitudinal
reinforcement. This improvement can be clearly understood by imagining the bars as parallel
springs. As the number of bars increased, the overall stiffness also increased, thereby lowering
the deflection after cracking, limiting the crack width, and decreasing the strain in the
reinforcement. Yoo et al. [28] reported that the flexural stiffness increased with increasing
longitudinal rigidity (A*fEf*) and suggested that the reinforcement ratio should be increased in
order to control crack width effectively.

17
on the strength of FRP-reinforced concrete beams could be fully realised when ρ*f* is increased
three to four times.

**4.3. Influence of the Anchorage System **

The strength and serviceability performance of HG-RGC was nearly comparable to that of SG-RGC. This can be expected since the straight and headed bars were fully bonded in the geopolymer concrete, thereby yielding similar results. As reported by Maranan et al. [31], the bond strength of the straight and headed GFRP bars approached similar performances as the embedment length increased. Thus, it can be deduced that a composite action can be achieved between the straight bars and the geopolymer concrete by fully embedding the bars in the geopolymer concrete and that the friction and mechanical interlock resistance provided by the sand coating were sufficient to produce a composite action between the GFRP bars and the geopolymer concrete.

**4.4. Comparison with Current Design Provisions **

In this study, the empirical equations recommended by the CSA S806-12 and ACI 440.R-06
were employed to assess the strength and serviceability performance of SG-RGC and
HG-RGC, while the ACI 318-14 code was adapted for the DS-RGC beam. Using Equation 7, the
theoretical cracking moments, M*cr-theo*, based on CSA and ACI are 11.1 kN-m and 11.5 kN-m,
respectively. The f*r* was calculated from Equation 8 for the CSA code. Equation 9, on the other
hand, was used for the ACI codes with the assumption that λ is equivalent to 1.0. Generally,
the predicted values were relatively close to the experimental results, with the ACI code
providing a more conservative estimate.

18
by solving first the neutral axis location, c, from Equation 11 and then substituting this value
to Equation 12. For ACI 440.1R-06, the f*f* was calculated with Equation 13. On the other hand,
Equation 14, recommended by ACI 318-08, predicted the flexural capacity of DS-RGC at steel
yielding failure. Table 4 summarises the M*u-theo* of the tested beams. The values estimated
according to CSA S806-12 were higher than those predicted by ACI 440.1R-06, owing to the
*β1* factor and the higher ε’*cu* normally assumed in CSA (0.0035) compared to ACI (0.003).
Generally, both prediction equations underestimated the flexural capacity of all the tested
beams. The average theoretical strengths of the beams based on ACI 440.1R-06 and CSA
S806-12 are 76 % and 81%, respectively, of the experimental flexural strengths. Generally, this
finding can be attributed to three major factors. First, the assumed concrete compressive strains
(0.003~0.0035) used in the predictions are lower compared to the actual strain recorded during
the flexural tests, which reached higher values ranging from 0.0042 to 0.0048. Second, the
prediction equations did not include the contribution of the reinforcement in the compression
zone. Finally, the confinement effect due to the lateral ties (stirrups) provided in the pure
bending-moment zone were not considered.

19
in terms of deflection limit L/240. Table 5 also shows the predicted midspan deflection at
failure Δ*u-theo* of the tested beams. Again, both design equations did not conservatively estimate
beam *Δu-theo*. The degree of underestimation increased with an increase in the applied load,
owing to the overestimation of the tension stiffening parameter. Furthermore, these equations
were developed from a full-interaction analysis of transformed section wherein it is assumed
that no slip between the concrete and the reinforcements, which is not the case in the actual
condition. Visintin et al. [38] suggested the use of partial-interaction theory that allows the slip
between the reinforcement and concrete. Thus, considering the mentioned factors and the
concept of partial-interaction theory, an appropriate prediction equation is now being
developed for the proposed system.

**4.5. Comparison between the Experimental Results and the FRP-Reinforced Concrete **

**Beams **

20 geopolymer concrete core, thereby increasing the beam strength and ductility. Lastly, the tensile strength (617 MPa to 695 MPa) and modulus of elasticity (40 GPa to 55 GPa) of the GFRP bars used in the previous studies were lower than the tensile strength and the modulus of elasticity of the bars used in this study. The high compressive strain capacity of geopolymer concrete was coupled with GFRP bars having a high tensile strength resulted in a beam with high flexural strength and ductility. Table 6 shows the amount of tensile strains in the bottom GFRP bars at geopolymer concrete crushing failure. These strains translate to a tensile stresses than can reach up to 892 MPa. If the beams were reinforced with GFRP bars of lower tensile strength, the beams will fail earlier due to bar rupture, yielding lower flexural strengths.

**5. Conclusion **

This paper presented an assessment of the strength and serviceability of geopolymer concrete beams reinforced with GFRP bars subjected to four-point static bending testing. Based on the experimental results and theoretical predictions, the following can be concluded:

The load-deflection curves of the beams with GFRP bars consist primarily of three

segments, including a steep linear branch that corresponds to cracked response of the beam; linear and nonlinear segments with reduced slope that represent the cracked response of the beam; and a nonlinear segment after the crushing failure of the geopolymer concrete.

The beams reinforced with GFRP bars failed by concrete crushing failure, since they

were designed as over-reinforced, while the under-reinforced beam with steel bars failed due to reinforcement yielding.

The bending-moment capacities at concrete crushing failure of GFRP-reinforced

21

The uncracked response of all the tested beams was similar since, at this stage, the

flexural performance of the beam was governed by the geopolymer concrete properties.

For beams with similar reinforcement ratios, it appears that the GFRP bar nominal

diameter had insignificant effect on their flexural behaviour.

Increasing the reinforcement ratio would enhance the serviceability performance of the

GFRP-reinforced geopolymer concrete beams. Doubling the reinforcement ratio, however, did not increase the beams load-carrying capacity at concrete crushing failure since the beams were designed as over-reinforced and therefore, their strength would be dependent on the geopolymer concrete strength and not by bar rupture.

The mechanical interlock and friction force resistance provided by the sand coating,

bonded on the surface of the GFRP bars, were found to be adequate to secure a composite action between the bars and the geopolymer concrete.

Generally, both the ACI-440.1R-06 and CSA S806-12 prediction equations

underestimated the flexural capacity of GFRP-reinforced geopolymer concrete beams. This may be due to the following factors: lower compressive strains used in the prediction (0.003 and 0.0035, respectively) compared to the actual strains (0.0042~0.0048); neglection of the compression strength contribution of top GFRP bars; and exclusion of the confinement effect of stirrups located in the pure bending-moment zone.

The bending-moment capacity of GFRP-reinforced geopolymer concrete beams seems

to be higher than that of GFRP-reinforced concrete beams mainly because of the enhanced mechanical properties of the geopolymer concrete compared to the conventional concrete of the same grade. Further investigations, however, are needed to support this generalisation.

22

*a * beam shear span

*b * beam width

*c * neutral axis depth from the top compression fibre

*d * beam effective depth

*Ec* modulus of elasticity of the geopolymer concrete
*Ef* modulus of elasticity of the GFRP bars

*Es* modulus of elasticity of the steel bars

*fr-exp* experimental modulus of rupture of the geopolymer concrete

*fr-theo* theoretical modulus of rupture of the geopolymer concrete

*ffu* guaranteed tensile strength of the GFRP bars
*ff* tensile stress in the GFRP bars

*fy* yield strength of the steel bars

*f'c* compressive strength of the geopolymer concrete

*h * beam total depth

*Icr* cracked moment of inertia
*Ie* effective moment of inertia
*Ig* gross moment of inertia

*L * beam clear span

*Lg* uncracked beam length

*Ma.* actual bending-moment

*Mcr.* cracking moment

*Mcr-exp* experimental cracking moment

*Mcr-theo* theoretical cracking moment

*Mpeak-exp* experimental peak bending-moment

23

*Mu-exp* experimental bending-moment at geopolymer concrete crushing failure

*Mu-theo* theoretical bending-moment at geopolymer concrete crushing failure

*Y * neutral axis depth from the top compression fibre

*P * applied load

*α1* constant variable

*β1* constant variable

*Δ * midspan deflection

*Δpeak-exp* experimental midspan deflection at peak

*Δs-exp* experimental midspan deflection at service load

*Δu-exp* experimental midspan deflection at concrete crushing failure

*Δu-theo* theoretical midspan deflection at concrete crushing failure

*Δunl-exp* experimental midspan deflection at the unloaded phase

*ε'cu* usable compressive strain of the geopolymer concrete

*ε'cu-exp* experimental compressive strain at geopolymer concrete crushing failure

*ε'c* peak strain, compressive strain at peak stress of the geopolymer concrete
*εfu* ultimate usable tensile strain of the GFRP bars

*η * constant variable

*Øf* nominal diameter of the GFRP bars
*Øs* diameter of the steel bars

*ρb* balanced reinforcement ratio of the steel bars
*ρf* reinforcement ratio of the GFRP bars

*ρfb* balanced reinforcement ratio of the GFRP bars
*ρs* reinforcement ratio of the steel bars

25
**References **

[1] Ascione L, Razaqpur AG, Spadea S. Effectiveness of FRP stirrups in concrete beams subject to shear. In: El-Hacha R, editor. The 7th Interntional Conference on FRP Composites in Civil Engineering (CICE 2014). Vancouver, Canada: International Institute for FRP in Construction (IIFC); 2014. p. 368-73.

[2] Hardjito D, Wallah SE, Sumajouw DMJ, Rangan BV. On the development of fly ash-based geopolymer concrete ACI Materials Journal. 2004;101:467-72.

[3] Sumajouw DMJ, Hardjito D, Wallah SE, Rangan BV. Fly-ash based geopolymer concrete: Study of slender columns. Journal of Materials Science. 2007;42:3124-30.

[4] Fernandez-Jimenez AM, Polomo A, Lopez-Hombrados C. Engineering properties of alkali-activated fly ash concrete. ACI Materials Journal. 2006;103:251-7.

[5] Sofi M, Deventer JSJv, Mendis PA, Lukey GC. Engineering properties of inorganic polymer concretes (IPCs). Cement and Concrete Research. 2007;42:3107-16.

[6] Faza SS, Gangarao HVS. Theoretical and experimental correlation of behaviour of concrete beams reinforced with fibre reinforced plastic rebars American Concrete Institute. 1993;SP138:599-614.

[7] Karbhari V, Seible F. Fiber-reinforced polymer composites for civil infrastructure in the USA. Structural Engineering International. 1999;9:186-94.

[8] V-ROD. V-ROD® Australia: Composite reinforcing rod. Inconmat Australia.

[9] Abraham R, Raj S D, Abraham V. Strength and behaviour of geopolymer concrete beams. International Journal of Innovative Research in Science, Engineering and Technology. 2013;2:159-66.

26 [11] Matos B, Correia JR, Castro LMS, Franca P. Structural response of hyperstatic concrete beams reinforced with GFRP bars: Effect of increasing concrete confinement. Composite Structures. 2012;94:1200-10.

[12] Mousavi SR, Esfahani MR. Effective moment of inertia prediction of FRP-reinforced concrete beams based on experimental results. ASCE Journal of Composites for Construction. 2012;16.

[13] Nawy EG, Neuwerth GE, Philips CJ. Behaviour of fibre glass reinforced concrete beams. ASCE Journal of Structural Division. 1971;97:2203-15.

[14] Noel M, Soudki K. Estimation of the crack width and deformation of FRP-reinforced concrete flexural members with and without transverse shear reinforcement. Engineering Structures. 2014;59:393-8.

[15] Adam MA, Said M, Mahmoud AA, Shanour AS. Analytical and experimental flexural behavior of concrete beams reinforced with glass fiber reinforced polymer bars. Construction and Building Materials. 2015;84:354-66.

[16] Au FTK, Du JS. Deformability of concrete beams with unbonded FRP tendons. Engineering Structures. 2008;30:3764-70.

[17] Rangan BV, Sumajouw D, Wallah S, Hardjito D. Reinforced low-calcium fly ash-based geopolymer concrete beams and columns. Our World in Concrete and Structures. Singapore: CI-Premier PTE LTD; 2006.

[18] Dattatreya JK, Rajamane NP, Sabitha D, Ambily PS, Nataraja MC. Flexural behaviour of reinforced geopolymer concrete beams. International Journal of Civil and Structural Engineering. 2011;2:138-59.

27 [20] Maranan GB, Manalo AC, Karunasena W, Benmokrane B. Bond Stress-Slip: Case of GFRP bars in Geopolymer Concrete. ASCE Journal of Materials in Civil Engineering. 2014. [21] Pultrall. V-ROD FRP reinforcing bars data sheet. 2012.

[22] CSA. Design and construction of building structures with fibre-reinforced polymers. CSA S806-12. Mississauga, Ontario, Canada: Canadian Standards Association; 2012.

[23] ACI. Guide for the design and construction of structural concrete reinforced with FRP bars. ACI 4401R-06. Farmington Hills, MI, USA: American Concrete Institute; 2006.

[24] ACI. Building code requirements for structural concrete. ACI 318-08. Farmington Hills, MI, USA: American Concrete Institute; 2008.

[25] El-Nemr A, Ahmed EA, Benmokrane B. Flexural behavior and serviceability of normal- and high-strength concrete beams reinforced with glass fiber-reinforced polymer bars. ACI Structural Journal. 2013;110:1077-88.

[26] Kassem C, Farghaly AS, Benmokrane B. Evaluation of flexural behavior and serviceability performance of concrete beams reinforced with FRP bars. ASCE Journal of Composites for Construction. 2011;15:682-95.

[27] Balendran RV, Tang WE, Leung HY, Nadeem A. Flexural behaviour of sand coated glass-fibre reinforced polymer (GFRP) bars in concrete. Our World in Concrete and Structures. Singapore2004. p. 203-12.

[28] Razaqpur AG, Svecova D, Cheung MS. Strength and deformations of FRP reinforced flat slab structures. In: Taerwe L, editor. Proceedings of the Second International RILEM Symposium (FRPRCS-2): E & FN Spon; 1995.

28 [30] Yoo DY, Shin HO, Kwon KY, Yoon YS. Structural behavior of UHPFRC beams according to reinforcement ratio of internal GFRP bar. In: El-Haacha R, editor. The 7th International Conference on FRP Composites in Civil Engineering (CICE 2014). Vancouver, British Columbia, Canada: International Institute for FRP in Construction (IIFC); 2014. [31] Maranan GB, Manalo AC, Karunasena W, Benmokrane B. Pullout behaviour of GFRP bars with anchor head in geopolymer concrete Composite Structures. 2015;132:1113-21. [32] Gangarao HVS, Tally N, Vijay PV. Reinforced concrete design with FRP composites: CRC Press; 2007.

[33] Kakizawa T, Ohno S, Yonewa T. Flexural behavior and energy absorption of carbon FRP reinforced concrete beams. American Concrete Institute. 1993;138:585-98.

[34] ISIS. Reinforcing concrete structures with fibre-reinforced polymers. ISIS Design Manual No 3. Winnipeg, Manitoba, Canada: Intelligent Sensing for Innovative Structures (ISIS) Canada; 2006.

[35] Bischoff PH, Gross S, Ospina CE. The story behind the proposed changes to the ACI 440 deflection requirements for FRP-reinforced concrete. In: Ospina C, Bischoff PH, Alkhrdaji T, editors. Serviceability of concrete members reinforced with internal/external FRP reinforcement. Farmington Hills, MI: American Concrete Institute; 2009. p. 53-76.

[36] Ehsani MR, Saadatmanesh H, Tao S. Bond behaviour of deformed GFRP rebars. Journal of Composite Materials. 1997;31:1413-30.

[37] Masmoudi R, Benmokrane B, Chaallal O. Cracking behaviour of concrete beams reinforced with FRP bars. Canadian Journal of Civil Engineering. 1996;23:1172-9.

[38] Visintin P, Oehlers DJ, Muhamad R, Wu C. Partial-interaction Short Term Serviceability Deflection of RC Beams. Engineering Structures. 2013;56:993-1006.

29 [40] Visintin P, Oehlers DJ, Wu C, Haskett M. A mechanics solution for hinges in RC beams with multiple cracks. Engineering Structures. 2012;36:61-9.

[41] Oehlers DJ, Ali MSM, Haskett M, Lucas W, Muhamad R, Visintin P. FRP-Reinforced concrete beams: Unified approach based on IC theory. Journal of Composites for Construction. 2011;15:3-293-303.

[42] Marti P, Alvarez M, Kaufmann W, Sigrist V. Tension chord model for structural concrete. Structural Engineering International. 1998;8:287-98.

[43] Muhamad R, Ali MSM, Oehlers DJ, Sheikh AH. Load-slip relationship of tension reinforcement in reinforced concrete members. Engineering Structures. 2011;33:1098-106. [44] Kara IF, Ashour AF. Flexural performance of FRP reinforced concrete beams. Composite Structures. 2012;94:1616-25.